I just annealed about 100 30-30 cases for my 788 Rem. I was taught to place the cases in water, about half way up, heat with a propane torch until the necks turn a dull red, and knock them over into the water. I see some don't tip the cases over into the water, letting them cool naturally, and some shooters use other methods to anneal, such as holding the case in hand, while heating, and when too hot to hold they are done. Is there a best way to do this? Or doesn't it matter. I am sure this has likely been discussed before. Just would like opinions, for future reference.
Annealing Rifle Brass
- 523 Views
- Last Post yesterday
- Topic Is Solved
Thanks Jeff, but that's a little above my price range.
Actually copper bearing alloys are annealed by heating followed by a quench. Why this will harden steels but soften copper and brass I don't recall right now, but, it is considerably better to quench the case rather than just let it cool without knocking it over.
Goes without saying that you take measures to make damn sure you don't try to anneal a case with a live primer, and as always eye protection is a damn good idea.
I definitely deprime before annealing. I don't like sudden noises.
Annealing brass has nothing to do about water quench or time. The only factor in temperature. The only reason to put cases into the water is to insure that the case head never gets about 100 Celsius.
Do you know about where on your curve the factories anneal new brass after case forming?
John, Nope and there may not be any standard. Ed Harris may know from his time at Ruger and work with the military. Ric
Talled to Starline about annealing the day before the last CBA Nationals. I had several questions and their production engineer spent the time with me. I was greatly appreciative of his time and knowledge.
Given: My uncles toured the W-W Alton factory based on their experience as competition shooters and reloaders. The plant officials were not eager to give tours until they realized the two brothers shot thousands of rounds each year. They noticed annealing was done on a line in gas jets and the line continued for several feet before dropping off to air dry.
My first question concerned air or water dry. They were strong on water quench for the reloader because this is a reliable constant. They have gauges to sense the temperature and monitor these all day long. Either method is workable, but the average reloader does not have the gauging to correctly monitor.
My second question concerned correct temperature gauging. I mentioned I was using welder temperature sticks to gauge the heat. They stated using Tempilaq for heat sensing rather than welding sticks. They felt Tempilaq is easier to apply and more sensitive than welding sticks.
The next discussion concerned my frustration at making .25-20 brass from .32-20. I told them my first lot of their .32-20 formed to .25-20 easily several years, but the recent lot gave me three collapsed shoulders out of the first ten. I stopped knowing I was going to be able to talk to them within two months. They said their brass is shipped from the factory in a range of hardness, I possibly had the extremes of the upper and lower hardness limits. They stated they were having the same problem forming .25-20 as an experiment and the production was not economically feasible for a production facility. They recommended an intermediate step and discussion soon found I had a 7mm BR die that would work.
Tomorrow morning begins the quest to anneal 300+ .308 Lapua brass for Alice this coming season as it has work hardened. Then 300 .32-20 brass for sizing to .25-20 to assure adequate brass for the coming year of competition and the Quarter-Bore matches. .
Country boy from Western Illinois, living in the Magical Pacific Northwest
I form .17 Mashburn Bee brass from .218 Bee--25-20 & from 32-20 also. I made all of my forming dies myself. and after lots of testing and tweaking of equipment I can turn out a near perfect case even before it is fireformed. This is quite a change in case dimensions and shape and you have to leave the head and web alone. I don't care what people tell you to do-use the water quinch method. It's nice to talk about high tech equipment and sensors and such but how many people have access to this equipment. Templac costs money and takes time to apply. I have been annealing cases for about 55 years and have never ruined a case. My trick to getting the right heat color is- I turn nearly all of the lights off in the shop and get my water pan over in a dim corner and start too work. It is so much easier to read the colors in dim light. Most of my case forming is for wildcat calibers so I anneal a little below the shoulder. When my water starts to get hot I pour it out and put in fresh cool water. As the water gets hot it will effect the degree of hardness on the case that you are working on.Keeping the water froom getting too hot will keep you from over heating the case head and webb.
You are absolutely correct about new cases being drawn out to different degrees and different brands will vary from another.
You can take what I just told you to the bank
David a. Cogburn
Mashburn said: " Keeping the water froom getting too hot will keep you from over heating the case head and webb.
The case heads and webbs wouldn't seem to be in much danger. Even boiling water in the open only gets to 212 F and even the slightest annealing doesn't start until the temperature is over 400F (Ric's curves)? Are the curves wrong?
I use a circular head torch that I bought from Todd Kindler (the reloading den) years ago. This could be easily made by drilling holes in a Cooper pipe and bending in a couple inch circle.
I turn the lights off and when I see the case just start to glow I deduct 1 second from my timmer.
I do not use water. The case head never gets near hot enough to cause problems. I look for the discoloration of the case like factory cases.
I work @ W-W Oxford. I can tell you my process is much tamer than the factory
John, Unless the P.E. metallurgy site is in error, I would trust that graph. Ric
getting a constant temp on the brass is very important. Going by looking for color change gives one a big variable in temp of the brass being annealed. I have for years used Tempilaq liquid from Brownells. This is a temp sensitive liquid that one brush on the inside of he neck. The case is rotated in the flame and when the Tempilaq turns clear you have reached the temp that it is specific for. It comes in different temp ranges. Do a couple of cases and note the time needed for the Tempilaq to become clear, on subsequent cases keep in the flame for the amount of seconds from the trial cases then remove when it becomes clear.
A couple years ago I went to using the Anneal-Rite system https://cartridgeanneal.com/ . The only difference is I use the Tempilaq only once, counting till it changes color or melts at 750 degrees. I then keep a log of the time or count to use for future annealing of the same cartridge. It is a pretty fool proof system and I can do about 10-20 cases a minute depending on the time for each case which is usually between 2-4 seconds.
David Reiss - NRA Life Member & PSC Range Member Retired Police Firearms Instructor/Armorer
-Services: Wars Fought, Uprisings Quelled, Bars Emptied, Revolutions Started, Tigers Tamed, Assassinations Plotted, Women Seduced, Governments Run, Gun Appraisals, Lost Treasure Found.
- Also deal in: Land, Banjos, Nails, Firearms, Manure, Fly Swatters, Used Cars, Whisky, Racing Forms, Rare Antiquities, Lead, Used Keyboard Keys, Good Dogs, Pith Helmets & Zulu Headdresses. .
I've had great luck using the "Fred Barker Candle annealing method"
Just read the Fred Barker method. That is so simple even I could do it. Now I just have to talk my wife into some romantic candle light time and I can get twice as much done!
- All Categories
- General Polls
- Contact Us w/ Forum Issues
- Welcome to The Cast Bullet Association Forum
- Bullet Casting
Guns & Shooting
- AR Platform
- TC Contenders & Other Single Shot Handguns
- Informal Matches & Other Shooting Events
- Gunsmithing Tips
- Gun Cleaning & Maintenance
- Benchrest Cast Bullet Shooting
- Military Bench Rest Cast Bullet Shooting
- Silhouette Shooting
- Postal Match Cast Bullet Shooting
- Factory Guns
- Black Powder Cartridge
- Hand Guns
- Lever Guns
- Single Shot Rifles
- Bolt Action Rifles
- Military Surplus Rifles
- Plinkers Hollow
- Buy, Sell or Trade
- Other Information & Reference